LMucko/crystallography-open-database huggingface dataset:
Electric conductivity of Fe2SiO4-Fe3O4 spinel solid solutions Sample: Fe(3-x)SixO4, x = 1.000, synthesized at 1200 C, 10 GPa
Yamanaka, T.; Shimazu, H.; Ota, K.; Physics and Chemistry of Minerals 28 (2001) 110–118; doi:10.1007/s002690000137

data_9006925
_publ_section_title
;
 Electric conductivity of Fe2SiO4-Fe3O4 spinel solid solutions
 Sample: Fe(3-x)SixO4, x = 1.000, synthesized at 1200 C, 10 GPa
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              110
_journal_page_last               118
_journal_paper_doi               10.1007/s002690000137
_journal_volume                  28
_journal_year                    2001
_chemical_compound_source        Synthetic
_chemical_formula_structural     Fe2SiO4
_chemical_formula_sum            'Fe2 O4 Si'
_chemical_name_mineral           Ahrensite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2374
_cell_length_b                   8.2374
_cell_length_c                   8.2374
_cell_formula_units_Z            8
_cell_volume                     558.947
_database_code_amcsd             0008507
_exptl_crystal_density_diffrn    4.843
_exptl_crystal_pressure_history  'synthesized at 1200 C, 10 GPa'
_exptl_crystal_thermal_history   'synthesized at 1200 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Fe2 Si) O4'
_cod_database_code               9006925
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 297 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006926
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 297 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8444
_cell_length_b                   7.8444
_cell_length_c                   5.0265
_cell_formula_units_Z            2
_cell_volume                     309.304
_database_code_amcsd             0008508
_diffrn_ambient_temperature      297
_exptl_crystal_density_diffrn    3.299
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006926
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 393 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006927
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 393 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8507
_cell_length_b                   7.8507
_cell_length_c                   5.0281
_cell_formula_units_Z            2
_cell_volume                     309.899
_database_code_amcsd             0008509
_diffrn_ambient_temperature      393
_exptl_crystal_density_diffrn    3.293
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006927
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 468 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006928
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 468 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8563
_cell_length_b                   7.8563
_cell_length_c                   5.0294
_cell_formula_units_Z            2
_cell_volume                     310.422
_database_code_amcsd             0008510
_diffrn_ambient_temperature      468
_exptl_crystal_density_diffrn    3.287
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006928
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 493 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006929
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 493 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8590
_cell_length_b                   7.8590
_cell_length_c                   5.0260
_cell_formula_units_Z            2
_cell_volume                     310.425
_database_code_amcsd             0008511
_diffrn_ambient_temperature      493
_exptl_crystal_density_diffrn    3.287
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006929
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 503 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006930
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 503 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8591
_cell_length_b                   7.8591
_cell_length_c                   5.0258
_cell_formula_units_Z            2
_cell_volume                     310.421
_database_code_amcsd             0008512
_diffrn_ambient_temperature      503
_exptl_crystal_density_diffrn    3.287
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006930
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 533 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006931
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 533 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8615
_cell_length_b                   7.8615
_cell_length_c                   5.0268
_cell_formula_units_Z            2
_cell_volume                     310.672
_database_code_amcsd             0008513
_diffrn_ambient_temperature      533
_exptl_crystal_density_diffrn    3.285
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006931
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 573 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006932
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 573 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8656
_cell_length_b                   7.8656
_cell_length_c                   5.0289
_cell_formula_units_Z            2
_cell_volume                     311.126
_database_code_amcsd             0008514
_diffrn_ambient_temperature      573
_exptl_crystal_density_diffrn    3.280
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006932
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 673 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006933
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 673 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8732
_cell_length_b                   7.8732
_cell_length_c                   5.0336
_cell_formula_units_Z            2
_cell_volume                     312.019
_database_code_amcsd             0008515
_diffrn_ambient_temperature      673
_exptl_crystal_density_diffrn    3.270
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006933
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 773 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006934
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 773 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_structural     Ca2CoSi2O7
_chemical_formula_sum            'Ca2 Co O7 Si2'
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8815
_cell_length_b                   7.8815
_cell_length_c                   5.0387
_cell_formula_units_Z            2
_cell_volume                     312.994
_database_code_amcsd             0008516
_diffrn_ambient_temperature      773
_exptl_crystal_density_diffrn    3.260
_cod_original_formula_sum        'Co Ca2 Si2 O7'
_cod_database_code               9006934
_amcsd_formula_title             Ca2CoSi2O7
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 297 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006935
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 297 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Ca2 Mg O7 Si2'
_chemical_name_mineral           Akermanite
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8348
_cell_length_b                   7.8348
_cell_length_c                   5.0087
_cell_formula_units_Z            2
_cell_volume                     307.454
_database_code_amcsd             0008517
_diffrn_ambient_temperature      297
_exptl_crystal_density_diffrn    2.945
_cod_original_formula_sum        'Mg Ca2 Si2 O7'
_cod_database_code               9006935
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 348 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006936
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 348 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Ca2 Mg O7 Si2'
_chemical_name_mineral           Akermanite
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8387
_cell_length_b                   7.8387
_cell_length_c                   5.0079
_cell_formula_units_Z            2
_cell_volume                     307.712
_database_code_amcsd             0008518
_diffrn_ambient_temperature      348
_exptl_crystal_density_diffrn    2.942
_cod_original_cell_volume        307.711
_cod_original_formula_sum        'Mg Ca2 Si2 O7'
_cod_database_code               9006936
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 359.4 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006937
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 359.4 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Ca2 Mg O7 Si2'
_chemical_name_mineral           Akermanite
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8387
_cell_length_b                   7.8387
_cell_length_c                   5.0072
_cell_formula_units_Z            2
_cell_volume                     307.668
_database_code_amcsd             0008519
_diffrn_ambient_temperature      359.4
_exptl_crystal_density_diffrn    2.943
_cod_original_formula_sum        'Mg Ca2 Si2 O7'
_cod_database_code               9006937
Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of diffuse streaks at high temperature Sample: T = 359.7 K Melilite group
Kusaka, K.; Hagiya, K.; Ohmasa, M.; Okano, Y.; Mukai, M.; Iishi, K.; Haga, N.; Physics and Chemistry of Minerals 28 (2001) 150–166; doi:10.1007/s002690000147

data_9006938
_publ_section_title
;Determination of structures of Ca2CoSi2O7, Ca2MgSi2O7, and
 Ca2(Mg.55Fe.45)Si2O7 in incommensurate and normal phases and observation of
 diffuse streaks at high temperature Sample: T = 359.7 K Melilite group
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              150
_journal_page_last               166
_journal_paper_doi               10.1007/s002690000147
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Ca2 Mg O7 Si2'
_chemical_name_mineral           Akermanite
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8398
_cell_length_b                   7.8398
_cell_length_c                   5.0058
_cell_formula_units_Z            2
_cell_volume                     307.669
_database_code_amcsd             0008520
_diffrn_ambient_temperature      359.7
_exptl_crystal_density_diffrn    2.943
_cod_original_formula_sum        'Mg Ca2 Si2 O7'
_cod_database_code               9006938